From Online Dictionary of Crystallography
Revision as of 15:54, 2 April 2017 by MassimoNespolo (LF missing)
Indices de Weber (Fr). Índices de Weber (Sp). Indici di Weber (It). ウェーバー指数 (Ja)
For trigonal and hexagonal crystals, the Miller indices are conveniently replaced by the Bravais-Miller indices which make reference to a four-axes setting. For lattice directions, a similar extension to a four-axes axial setting exists, known as the Weber indices, UVTW.
Let A1,A2,A3,C be the four hexagonal axes, written as capital letter to avoid any possible confusion with the rhombohedral axes a1,a2,a3, and let be uvw and UVTW the indices of a direction with respect to A1,A2,C or A1,A2,A3,C respectively. For a given direction the following identity must hold:
uA1 + vA2 + wC = UA1 + VA2 + TA3 + WC.
Now, because in the two-dimensional (001) plane only two of the three axes are linearly independent, the following identity can be established:
A1 + A2 + A3 = 0 --> A3 = -(A1 + A2).
A similar relation holds for the Weber indices:
U + V + T = 0.
Substituting the above identities, one immediately gets:
uA1 + vA2 + wC = UA1 + VA2 - T(A1 + A2 ) + WC
uA1 + vA2 + wC = (U-T)A1 + (V-T)A2 + WC
u = U-T; v = V-T; w = W
U + V + T = 0 --> T = -(U+V)
u = 2U+V; v = U+2V; w = W
To find the opposite relations, one has simply to subtract the second equation from the first multiplied by two and vice versa:
2u-v = 3U --> U = (2u-v)/3
-u+2v = 3V --> V = (2v-u)/3
T = -(U+V) = -(u+v)/3.
The Weber indices of the direction perpendicular to a lattice plane are the same as the Bravais-Miller indices of that plane.